**THE EFFECT OF THE METHOD OF DETERMINATION OF**
**YOUNG’S MODULUS ON THE ESTIMATION OF FATIGUE**

**LIFE OF STRUCTURAL ELEMENTS**

Dariusz Boroński

*Department of Machine Design, University of Technology and Agriculture in Bydgoszcz*
*e-mail: daborpkm@atr.bydgoszcz.pl*

Cyclic loading of a material entails modifications of its properties. In
the paper, the problem of the influence of determination of the elasticity
*modulus E on calculations of the fatigue life of structural elements was*
presented. Different values of the modulus of elasticity obtained by
dif-ferent methods were used for modelling of cyclic stress-strain curves and
for analysis of local stresses and strains. In the calculations the strain-life
and energy-life approach was applied.

*Key words:* fatigue, modulus of elasticity, material properties

**1.** **Introduction**

The divergence between fatigue lives of structural elements determined
analytically and experimentally is the cause for continuous search for the ways
of modification of the existing methods of fatigue life calculation or creating
new ones. The research conducted at the Department of Machine Design at
the University of Technology and Agriculture in Bydgoszcz (UTA) (Szala and
*Boroński, 1995; Szala et al., 1994, 1998) has shown possible error sources in*
the prediction of the fatigue life, such as extrapolating life diagrams onto areas
*not included in fatigue tests or making use Young’s modulus E determined in*
a monotonic tension test in further calculations.

*Analysis of bibliographical data (e.g. Fatigue Design Handbook, 1988; *
*Ko-cańda and, Szala 1991; Roessle and Fatemi, 2000; Schijve, 2001; Smith et al.,*
1970; Topper and Lam, 1997) indicates common application of Young’s
*mo-dulus E with values assigned for monotonic loadings. The recently realised*
*research has given the possibility to check the variability of the modulus E*

according to the type of the material loading. This, in turn, has allowed one
to define the differences in the life estimation in the strain- and energy-based
*calculation methods, which are caused by alterations of the value E.*

**2.** **Theoretical basis**

When carrying out calculations using both the strain-based method and
the energy-based one (Szala, 1998), low-cycle material properties are used,
which are the basis for the estimation of the fatigue life diagrams (Fig. 1) and
*material-describing ones, e.g. stress-strain curves (Fig. 2). The modulus E*
appears in descriptions of these diagrams as a proportionality coefficient for
elastic strain components.

Fig. 1. Fatigue life diagrams

In the case of fatigue life diagram description in the strain approach using Manson-Coffin’s equation (Fig. 1a)

*εac= εap+ εae= ε0f(2Nf*)*c*+

*σ0*
*f*

*E(2Nf*)

*b* _{(2.1)}

*the modulus E does not affect the strain or life value. This is because fatigue*
tests according to standards (PN 84/H04334; ASTM 606-92) make use of the
*quotient σ0*

*f/E, and changes in the modulus E cause only changes in σ0f* with
*a constant value of σ0*

*f/E maintained, and thus the fatigue diagram remains*
unchanged.

The situation becomes different in the case of stress-strain curves de-scribing a material being loaded under variable conditions, described with

Ramberg-Osgood’s dependence
*ε = εe+ εp* =
*σ*
*E* +
*σ*
*K0*
* _{n0}*1
(2.2)
A standard research conducted to find the discussed characteristics gives only

*values describing the plastic element of the strain in dependence (2.2), i.e. K0*

*and n0*descrip-tion quantitatively.

_{. Therefore, the assumed modulus E may change the material }Fig. 2. Material properties (description in text)

A stress-strain diagram is used in the strain-based calculation method to determine the local strain and stress, e.g. using Neuber’s method (Neuber, 1961), see Fig. 2a, while in the energy-based calculation method, it may be used to describe the hysteresis loop (Fig. 2b).

Observation of the first and next load cycles (Fig. 3) allows one to notice
that a change in the material stiffness takes place, which causes a change in
*the modulus E. Hence, it may be agreed that there exist at least two E*
values: ”static” (monotonic) and ”dynamic”. Moreover, a precise analysis of
the hysteresis loop shows that it actually does not possess a linear-elastic
*segment, which increases the number of the possible-to-use E values by the*
static and linear approximation-based ones.

The ambiguity connected with the determination of the modulus of
elasti-city was presented among others in the work by Kandil (1999). The analysis of
*the methods of plastic strain determination using Young’s modulus E based*
on Standards BS 7270:1990; ASTM E606-92; ISO/DIS 12106; prEN 3988 for
specimens made of the Nimonic 101 nickel based superalloy showed differences
of over 30%. Moreover, different values of elasticity modulus for tension and
compression semicycles and its decrement together with an increase in the

Fig. 3. Hysteresis loops for 45 steel

strain were observed. The latter phenomena were described also in the work by Morestin and Boivin (1996) on investigations of specimens made of a plain steel and alloys A33, XC 38 and AU4G with a large cross-section and upon XE280D sheet metal type with a small cross-section.

*The aim of the paper is a quantitative analysis of the Young modulus E*
that depends on loading conditions (monotonic or cyclic variable), and in
the case of cyclic variable loading, depends also on the loading amplitude.
Moreover, differences in the estimated fatigue lives resulting from application
*of different moduli E are to be determined. The tests have been carried out*
*for three different materials. Additionally, changes in the modulus E during*
the fatigue tests have been observed.

**3.** **Experimental data**

The determination of the longitudinal elasticity modulus requires, accor-ding to ASTM E111 – 82/88 Standard, carrying out a monotonic tension test. The thus obtained stress dependence (force by cross-section) in function of strain is the basis for defining Young’s modulus. In the case of linear elastic materials, the modulus is a directional coefficient of a straight line describing the range of linear (proportional) material properties.

In the case of non-linear elastic materials, the tangent and secant moduli are introduced. The methods for their determination are shown in Fig. 4.

Fig. 4. Methods of determination of the elasticity modulus: (a) linear, (b) tangent, (c) secant

Three types of materials have been considered in the described research: Steel 45, Steel 30HGSA and Aluminium PA6.

The investigations were carried out in the Laboratory of Department of Machine Design at the University of Technology and Agriculture in Bydgoszcz using the INSTRON 8501 servohydraulic fatigue system with digital control system 8500. In the tests, standard specimens with round cross-sections were applied. The main dimensions of the specimens are shown in Fig. 5.

Fig. 5. Specimens used in the investigations

The INSTRON axial extensometers (collaborating with the strain channel of the loading control system) with two values of gauge length were used for strain measurements: 50 mm in the case of monotonic tension tests and 10 mm in the case of low cycle fatigue testing.

During the tests, the specimens were fastened by standard INSTRON hy-draulic grips.

The monotonic tension tests for all three materials revealed in the elastic
range nearly linear courses. The coefficients of the straight line correlation
*de-scribing the range were r*2* _{= 0.99993 for Steel 45, r}*2

_{∈ h0.9999, 1i for 30HGSA}*and r*2

*described by a second degree polynomial, and tangent moduli were*

_{∈ h0.9983, 0.9988i for Aluminium PA6. The obtained courses were also}determi-ned. Under those circumstances, the correlation coefficients were as follows:

*r*2* _{∈ h0.9999, 1i for Steel 45, r}*2

*2*

_{= 1 for 30HGSA and r}*Aluminium PA6.*

_{∈ h0.9997, 0.9999i for}*The obtained average moduli E are presented in Table 1. The variability*
coefficients determined according to ASTM and calculated on the basis of the
dependence
*V*1 = 100
s
1
*r*2 *− 1*
*K − 2* (3.1)

*where: K is the number of data pairs and r*2 _{is the correlation coefficient, are}
given there as well.

**Table 1**

Young’s modulus, Tangent modulus,

Material linear approxim., *V*1 polynomial approxim., *V*1
the average value the average value

45 Steel 222164 MPa 0.5% 226189 MPa *< 1.2%*

30HGSA Steel 208463 MPa *< 0.5%* 212920 MPa 0%
PA6 Aluminium 74237 MPa *< 1.58%* 83726 MPa *< 1%*

The hysteresis loops recorded during the fatigue tests in the low-cycle range
allowed one to determine the elasticity modulus, further called the dynamic
*modulus Ed*. Due to the fact that the hysteresis loop branches (Fig. 6) do not
possess the linear elastic part, the modulus of elasticity was decided to be
described according to the methodology shown in Fig. 4.

In determining the tangent modulus, the elastic part of the hysteresis loop
was approximated by a second degree polynomial with choosing such a
*frag-ment of the loop that the correlation coefficient was r*2 _{= 0.9999. Due to the}*fact that the secant value of the modulus E does not have a physical sense in*
the description of a cyclic strain diagram (the total strain must be on the right
side of the linear-elastic part), the directional coefficient of the straight line
approximating the initial segment of the hysteresis loop was agreed to be the
*value of the second modulus E (the same one as in the polynomial *
*approxi-mation), obtaining r*2 * _{> 0.9999. The thus obtained moduli E (average ones)}*
for different strain levels and for different materials are presented in Table 2.

**Table 2**

*Dynamic modulus Ed*, linear approximation

Material *Strain εac*% Average

0.35 0.5 0.8 1.0 2.0 value 45 Steel 165896 176302 180356 181431 174707 175738 30HGSA Steel 198774 190304 192406 192082 189422 192598 PA6 Aluminium 67304 73995 73330 70799 69660 71018

*Dynamic modulus Ed*, linear approximation

Material *Strain εac*% Average

0.35 0.5 0.8 1.0 2.0 value 45 Steel 209516 205587 209674 209369 201509 207131 30HGSA Steel 213649 208898 209842 209888 216278 211711 PA6 Aluminium 68337 76057 80365 74707 72727 74439

The obtained moduli are also presented in Fig. 7.

**4.** **Analysis of tests on the modulus** *E*

The analysis of the obtained values shows that the so-called dynamic
mo-dulus is lower than its static counterpart found in monotonic tests. Moreover,
the modulus changes depending upon the strain which is applied to the
spe-cimen. The changes are irregular, and the realisation of the fatigue tests on a
considerably greater number of strain levels would be required to determine a
*possible function describing the dependence of the modulus E on loading.*

*The modulus Ed* *differs with respect to E, at the maximum, by about 21%*
for Steel 45, about 8% for Steel 30HGSA and about 11% for Aluminium PA6.

*Fig. 7. Values of the modulus E; 1 – E (static) linear approximation, 2 – E (static)*
*tangent, 3 – Ed* *(dynamic) linear, 4 – Ed* *linear-mean, 5 – Ed* (dynamic) tangent,

*6 – Ed* tangent-mean

*Fig. 8. Exemplary courses of the modulus E for specimens made of the three tested*
materials

*During the research, variability of the modulus E in function of the *
num-ber of realised load cycles were observed as well. Figure 8 presents examples
*of moduli E for specimens made of the three tested materials, loaded in *
*sym-metric cycles of a constant strain value εac*. The comparison of the observed
values of the tangent modulus and of the modulus resulting from linear
appro-ximation in the case of steel specimens indicates increasingly weaker linearity

of the elastic hysteresis loop segment (an increase in the tangent modulus with a simultaneous decrease in the ”linear” modulus), and a decrease in the material stiffness. In the case of aluminium specimens, a minor increase in the modulus values occurred, which may indicate a growth in the material stiffness. The differences between the initial and final moduli were growing together with the intensification of the load applied to the specimens. For all the materials, the differences did not exceed 10%.

**5.** **Analysis of fatigue life calculations**

The determined, on the basis of tests, static and dynamic, values of the
*modulus E were used for calculation of the fatigue life of notched structural*
elements by means of the strain-based method (for the three materials) and
energy-based method (for 45 Steel).

In the case of the strain-based calculation method, the notched element was
modelled according to Neuber’s hypothesis (Fig. 2a), assuming in the material
*model description a stress-strain curve of different values of the modulus E.*
In the case of the energy-based calculation method, the plastic strain energy
was calculated by describing the hysteresis loop branch by means of a doubled
stress-strain curve (Fig. 2b) and Neuber’s local strain and stress analysis

*∆ε*
2 =
*∆σ*
*2E* +
*∆σ*
*2K0*
* _{n0}*1
(5.1)

*assuming different values of E.*

Low-cycle properties of the three tested materials, discussed in the works
*by Szala et al. (1998), were used in the calculations. These properties are*
presented in Table 3.
**Table 3**
Material *c* *b* *ε0*
*f*
*σ0*
*f* *K0* _{n}0_{C}_{0} * _{m}*
[MPa] [MPa]
45 Steel

*−0.43915 −0.11668 0.165836 1304 1436 0.226796 2.68604 −0.5933*

*30HGSA Steel −0.81030 −0.08716 2.139042 1660 1068 0.066426*

*PA6 Alumin. −0.84613 −0.10016 0.117573 894*797 0.085848

The stress-strain curves used in both methods and defined for different
*values of E are shown in Fig. 9. The diagram analysis indicates fairly low*

*Fig. 9. Stress-strain curves for different values of the modulus E*

*influence of variability of the modulus E on the qualitative course of the*
material modelling curve.

*For 45 Steel, the greatest stress differences equal about ∆σ = 40 MPa*
*for the strain ε = 0.1%, and in the case of strain of about ∆ε = 0.08% for*
*stresses from the range of σ ∈ h400, 440i MPa. This means that the maximum*
difference in the case of strain-based stress determination is about 20%, while
reciprocally, i.e. determining the strain on the grounds of stress the result may
differ by about 14.5%.

*For 30HGSA Steel, the greatest differences equal about ∆σ = 40 MPa*
*for the strain ε = 0.27% (8% difference), and in the case of strain of about*

*∆ε = 0.035% for stresses σ ∈ h620, 660i MPa (12% difference).*

*For PA6 Aluminium the greatest stress differences are about ∆σ = 50 MPa*
*for the strain range ε ∈ h0.3, 0.5i% (which gives the difference of about 24%),*

*and in the case of strain of about ∆ε = 0.1% for stresses σ ∈ h460, 520i MPa*
(difference by about 14.3%).

The changes of the analytically determined local strain and plastic strain
energy (the hysteresis energy) for the given range of variability of the
*mo-dulus E in a structural element made of 45 Steel are presented in Fig. 10.*
*Three values of the nominal stress S (200, 300 and 400 MPa) and two values*
*of the stress concentration factor Kt* (1.5, 2.5) were used in the calculations.
The differences in the local strains (Fig. 10a) were about 20%. In the case of
fatigue life calculations (Fig. 10b) it caused differences from 57 up to 100%.

Fig. 10. Changes of the local strain (a), plastic strain energy (c), fatigue life for strain-based calculations (b) and energy based calculations (d) for 45 Steel

Similarly, in the case of the energy based approach, the maximal differences
*of the plastic strain energy ∆W (Fig. 10c) for the analysed range of variability*

*of the modulus E were 13-23%, which entailed differences in the fatigue life*
(Fig. 10d) from 21 up to 38%.

Fig. 11. Changes of the local strain (a), fatigue life for strain-based calculations (b) for 30HGSA Steel

Fig. 12. Changes of the local strain (a), fatigue life for strain-based calculations (b) for PA6 Aluminium

The results of analogous strain-based calculations made for 30HGSA Steel and PA6 Aluminium are shown in Fig. 11 and Fig. 12. The differences in the prediction of the local strains and fatigue life for the three analysed materials are collected in Table 4.

**Table 4**
Differences of
Material *ε* *2Nf* *∆W* *Nc*
*εr/εm* *(2Nf*)*r/(2Nf*)*m* *∆Wr/∆Wm* *(Nc*)*r/(Nc*)*m*
[%] [%] [%] [%]
45 Steel 21-23 57-100 13-23 21-38
30HGSA Steel 9-10 23-104
PA6 Aluminium 15-17 27-130
*where subscript r = range, m = mean.*

**6.** **Conclusions**

On the basis of the conducted tests and calculations, several conclusions concerning the sensitivity of Young’s modulus to variable loads can be drawn:

*• cyclic loading in the range of loads producing plastic strains decreases*

Young’s modulus; in the conducted tests, the phenomenon was least visible in the case of Steel 30HGSA (tangent modulus), and most visible in the case of Steel 45 (linear approximation modulus),

*• the value of modulus obtained by the linear approximation decreases*

with the number of cycles which, with somewhat growing tendency of the tangent modulus, indicates increasingly weaker linearity of the elastic part of the hysteresis loop,

*• a too small number of the realised loading levels does not allow one to*

determine the influence of the loading amplitude on Young’s modulus.
*The subsequently made simulations, in which different moduli E were*
applied, allowed one to notice that the determination method did not
consi-derably affect the calculated local strains and plastic strain energy. However,
even a small variation of the local strain may cause big differences in the
fati-gue life when the strain-life approach is applied, especially for small values of
strain.

For the least advantageous case, for PA6 Aluminium, with the coefficient

*Kt* *= 1.5 and the nominal stress value S = 200 MPa, the difference in the*
*estimation of the fatigue life was ∆ = 130%.*

*In spite of this, it can be stated that making use of moduli E defined*
on the basis of the literature data (including handbooks) should not produce
significant errors in engineering calculations on the fatigue life of structural
elements.

The obtained calculation results indicate also the necessity of further search on the sources of errors that appear in various methods of determination of the fatigue life.

**References**

*1. Fatigue Design Handbook, 1988, II edition, Society of Automative Engineering*
2. Kandil F.A., 1999, Potential ambiguity in the determination of the plastic
* strain range component in LCF testing, International Journal of Fatigue, 21,*
1013-1018

*3. Kocańda S., Szala J., 1991, Podstawy obliczeń zmęczeniowych, PWN, *
War-szawa

4. Morestin F., Boivin M., 1996, On the necessity of taking into account the variation in the Young modulus with plastic strain in elastic-plastic software,

*Nuclear Engineering and Design***, 162, 107-116**

5. Neuber H., 1961, Theory of stress concentration for shear strained prismatical
*bodies with arbitrary non-linear stress-strain law, Journal of Applied *

*Mecha-nics***, 28, 544-550**

6. Roessle M.L., Fatemi A., 2000, Strain-controlled fatigue properties of steels
**and some simple approximations, International Journal of Fatigue, 22, 495-511***7. Schijve J., 2001, Fatigue of Structures and Materials, Kluwer Academic *

Pu-blishers, Dordrecht

8. Smith K.N., Watson P., Topper T.H., 1970, A stress-strain function for
**the fatigue of metals, Journal of Materials, JMLSA, 5, 4, 767-778**

*9. Szala J., 1998, Hipotezy sumowania uszkodzeń zmęczeniowych, Wydawnictwa*
Uczelniane ATR, Bydgoszcz

10. Szala J., Boroński D., 1995, Comparative analysis of experimental and
*cal-culated fatigue life of the 45 steel notched structural member, The Archive of*

*Mechanical Engineering***, 1-2, 111-123**

11. Szala J., Mroziński S., Boroński D., 1994, Fatigue life of machines parts in periodical and irregular loading conditions, KBN Report (State Committee for Scientific Research Grant No 7 1282 91 01)

12. Szala J., Mroziński S., Boroński D., 1998, Investigations of fatigue damage summing process in low-cycle fatigue range, KBN Report (State Committee for Scientific Research Grant No 7 T07A 035 08)

13. Topper T.H., Lam T.S., 1997, Effective strain-fatigue life data for variable
* amplitude fatigue, International Journal of Fatigue, 19, Supp. No. 1, 137-143*
14. Standard ASTM E606-92, Standard Practice for Strain-Controlled Fatigue

Te-sting

15. Standard ASTM E111 – 82/88: Determination of Young’s, Tangent, and Chord Modulus

16. Standard BS 7270:1990, Method for constant amplitude strain controlled fati-gue testing, British Standards Institution, 1990

17. Standard ISO/DIS 12106, Metallic materials fatigue testing – axial strain con-trolled method, 1998

18. Standard PN-84/H-04334, Badania niskocyklowego zmęczenia metali

19. Standard PrEN 3988:1998, Aerospace series, Test methods for metallic mate-rials – constant amplitude strain-controlled low cycle fatigue testing, AECMA, draft no. 2, 1998

**Wpływ sposobu określania wartości modułu** **E na obliczenia trwałości**

**zmęczeniowej elementów konstrukcyjnych**
Streszczenie

*W pracy przedstawiono analizę ilościowej zmienności modułu E w zależności od*
rodzaju obciążenia (monotonicznie i cyklicznie zmienne), a w przypadku obciążenia
cyklicznie zmiennego także od wartości amplitudy obciążenia. Ponadto wyznaczono
*różnicę szacowanych trwałości wynikającą z przyjęcia różnych wartości modułu E.*
Badania przeprowadzono dla trzech różnych materiałów. Dodatkowo obserwowano
*zmianę wartości modułu E w różnych okresach trwałości zmęczeniowej.*